# Resilience

Sumário:

The ability of a material to absorb energy when deformed elastically and to return it when unloaded is called resilience. This is usually measured by the modulus of resilience, which is the strain energy per unit volume required to stress the material from, zero stress to the yield stress. The toughness of a material is its ability to absorb energy in the plastic range. The ability to withstand occasional, stresses above the yield stress without fracturing is particularly desirable in parts such as freight-car couplings, gears, chains, and crane hooks. Toughness is a commonly used concept, which is difficult to pin down and define.

The ability of a material to absorb energy when deformed elastically and to return it when unloaded is called resilience. This is usually measured by the modulus of resilience, which is the strain energy per unit volume required to stress the material from, zero stress to the yield stress s. The strain energy per unit volume for uniaxial tension is

 (1)

From the above definition the modulus of resilience is

 (2)

This equation indicates that the ideal material for resisting energy loads in applications where the material must not undergo permanent distortion, such as mechanical springs, is having a high yield stress and a low modulus of elasticity. Table 1 gives some values of modulus of resilience for different materials.

Table 1. Modulus of resilience for various materials

 Material E, psi s0, psi Modulus of resilience, Ur Medium-carbon steel 30×106 45000 33,7 High-carbon spring steel 30×106 140000 320 Duraluminium 10,5×106 18000 17,0 Cooper 16×106 4000 5,3 Rubber 150 300 300 Acrylic polymer 0,5×106 2000 4,0

### Toughness

The toughness of a material is its ability to absorb energy in the plastic range. The ability to withstand occasional, stresses above the yield stress without fracturing is particularly desirable in parts such as freight-car couplings, gears, chains, and crane hooks. Toughness is a commonly used concept, which is difficult to pin down and define. One way of looking at toughness is to consider that it is the total area under the stress-strain curve. This area is an indication of the amount of work per unit volume, which can be done, on the material without causing it to rupture. Figure 1.2 shows the stress-strain curves for high- and low-toughness materials. The high-carbon spring steel has a higher yield strength and tensile strength than the medium-carbon structural steel. However, the structural steel is more ductile and has a greater total elongation. The total area under the stresstrain curve is greater for the structural steel, and therefore it is a tougher material. This illustrates that toughness is a parameter that comprises both strength and ductility. The crosshatched regions in Fig. 1 indicate the modulus of resilience for each steel. Because of its higher yield strength, the spring steel has the greater resilience.
Several mathematical approximations for the area under the stress-strain curve have been suggested. For ductile metals that have a stress-strain curve like that of the structural steel, the area under the curve can be approximated by either of the following equations:

 (3)

 (4)

For brittle materials the stress-strain curve is sometimes assumed to be a parabola, and the area under the curve is given by

 (5)

Figure 1. Comparison of stress-strain curves

All these relations are only approximations to the area under the stress-strain curves. Further, the curves do not represent the true behavior in the plastic range, since they are all based on the original area of the specimen.

## Procurar conhecimento básico

Colocar uma frase para procurar por:

 Procurar por Texto completo Palavras chaves Títulos Resumo

A Total Materia Extended Range inclui uma coleção única de curvas tensão-deformação e diagramas para os cálculos na faixa de plástico para milhares de ligas de metal, tratamentos térmicos e temperaturas de trabalho. Curvas tensão verdadeira e engenharia são dadas para várias taxas de deformação quando aplicável.

Encontrar um gráfico de tensão-deformação no banco de dados é simples e leva apenas alguns segundos.

Digite o material de interesse no campo de pesquisa rápida. Você pode, opcionalmente, limitar a sua pesquisa, especificando o país / padrão de escolha no campo designado e então, clique em Pesquisar.

Depois de selecionar o material de seu interesse, clique no link diagramas de tensão-deformação para visualizar os dados para o material selecionado. O número de disponíveis diagramas de tensão-deformação é exibido entre parênteses ao lado do link.

Porque as curvas tensão-deformação da Total Materia são neutras em especificações padrão, pode rever tensão-diagramas, clicando no link apropriado para qualquer um dos subgrupos.

Além das curvas de tensão-deformação a diferentes temperaturas, o stress e os dados de deformação são dadas em um formato tabular que é conveniente para a cópia para, por exemplo, um software CAE.

É também possível ver curvas tensão-deformação e dados para outras temperaturas de trabalho.

Para isso, basta inserir uma nova temperatura no 'Enter temperatura' campo dentro do intervalo definido.

Após clicar no botão Calcular, uma nova curva é plotada e valores na tabela agora correspondem com a temperatura que você definiu. Veja o exemplo abaixo de 250°C.

Para você é uma oportunidade de fazer um test drive na Total Materia, nós convidamos você a participar de uma comunidade de mais de 150.000 usuários registrados através da Total Materia Free Trial.